South African Journal of Industrial Engineering August 2015 Vol 26(2) pp 93-103
HEAT TREATMENT OF TI-6AL-4V PRODUCED BY LASERCUSING#
T. Becker1*, M. van Rooyen2 & D. Dimitrov3
1,2Department of Mechanical Engineering University of Stellenbosch, South Africa
3Department of Industrial Engineering University of Stellenbosch, South Africa
LaserCUSING is a selective laser melting (SLM) process that is capable of manufacturing parts by melting powder with heat input from a laser beam. LaserCUSING demonstrates potential for producing the intricate geometries specifically required for biomedical implants and aerospace applications. One main limitation to this form of rapid prototyping is the lack of published studies on the material performance of the resulting material. Studies of the materials performance are often complicated by dependence on several factors, including starting powder properties, laser parameters, and post-processing heat treatments. This study aims to investigate the mechanical properties of LaserCUSING-produced Ti-6Al-4V and its performance relative to the conventional wrought counterpart. A combination of conventional and LaserCUSING-tailored heat treatments is performed. The resulting microstructures are studied and linked to the properties obtained from hardness tests. The findings highlight that LaserCused Ti-6Al-4V is competitive with traditional materials, provided that optimal parameters are chosen and parts are subject to tailored post-processing. In the as-built condition, LaserCused Ti-6Al-4V displays superior strength and hardness as a result of a martensitic microstructure, and a poorer performance in ductility. However, the material performance can be improved using tailored heat treatments. Careful consideration must be given to suitable post-processing before application in critical components in the aerospace or biomedical industry can occur.
LaserCUSING is n selektiewe lasersmeltproses met die vermo om onderdele te vervaardig deur die smelt van poeier met hitte inset van n laserstraal. LaserCUSING toon die potensiaal om ingewikkelde geometrie benodig vir biomediese implantate en lugvaart toepassings, te produseer. Een van die hoof beperkings tot hierdie vorm van blits prototipering is die tekort aan gepubliseerde studies oor die materiaaleienskappe van die gevolglike materiaal. Studies van die materiaaleienskappe is dikwels verder gekompliseer as gevolg van die invloed van verskeie faktore, soos die aanvanklike poeier eienskappe, die laser parameters en hittebehandelings na die lasersmeltproses. Hierdie studie beoog om die meganiese eienskappe van Ti-6Al-4V wat met LaserCUSING geproduseer is, en die vertoning daarvan relatief tot n konvensionele bewerkte eweknie, te ondersoek. n Kombinasie van konvensionele en aangepaste hittebehandelings is toegepas. Die resulterende mikro-strukture is ondersoek en verwantskappe tot die resultate van hardheidstoetse is gevind. Die resultate toon dat die Ti-6Al-4V met tradisionele materiale kan kompeteer mits optimale parameters vooraf gekies word en dat onderdele aangepaste hittebehandelings ondergaan. Die Ti-6Al-4V toon beter sterkte en hardheid, maar het swakker smeebaarheid. Noukeurige oorweging vir verwerking na die lasersmelt is nodig voor die toepassing daarvan op kritiese komponente.
# This article is an extension of a paper presented at the 15th Annual International RAPDASA
conference held in Stellenbosch, South Africa in November 2014. * Corresponding author
The recent demand from industry to gain greater control of customised part manufacture using the combined strengths of computer aided design (CAD) and 3D printing methods has focused interest on additive manufacturing (AM) techniques. These layer-wise manufacturing methods support a market niche for components with shorter production times and intricate geometry details . Although applications were historically confined to the production of prototypes, modern methods extend to the manufacturing of tooling inserts, biomedical implants, mass-customised consumer products, aerospace components, and artwork [1-7]. Among the AM methods, selective laser melting (SLM) dominates applications in the industrial and academic sectors . Compared with conventional fabrication routes, SLM offers a range of benefits. The complete melting of the metallic powder particles results in a near-100 per cent dense product without the need for component-specific tooling . This results in reduced production time and maximises material utilisation. Additionally, the layer-by-layer control provides geometrical freedom, and allows the designer to focus more on the functionality of the part than on its manufacturability . One example of a commercial SLM method is LaserCUSING by CONCEPT Laser GmbH. The process uses a stochastic exposure scheme based on the island principle. Each powder layer is divided into islands that are laser-scanned, based on a random distribution. It is claimed that this strategy reduces the accumulation of residual stresses caused by steep temperature gradients . The starting material consists of single-component metallic powders generated by an atomisation process, and includes steel, aluminium, nickel-based, titanium, bronze, and precious-metal alloys. Possibly the most prominent candidate material for demonstrating the industrial potential of LaserCUSING manufactured components is the titanium alloy Ti-6Al-4V. This alloy has the majority market share of titanium products, and is known for its high strength-to-density ratios, corrosion resistance, and relatively high temperature capabilities [9,10]. The good biocompatibility properties of Ti-6Al-4V, combined with the geometrical flexibility of LaserCUSING, makes the alloy an attractive option for creating customised medical implants . The ability of SLM techniques to fabricate intricate cooling channels also extends the materials scope of applications to aero-engine turbine blades . Despite the successes of LaserCUSING and other SLM methods, a few problems are frequently encountered. One concern is the introduction of residual stresses due to the localised thermal input from the laser. These stresses, which can exceed the yield strength of the material, result from the temperature gradient mechanism in which previously solidified layers hinder the thermal expansion of the newly-formed areas . Residual stresses have been attributed to the degradation of mechanical properties, part distortion, and micro-crack formation [12,14,15]. Furthermore, 100 per cent density is often difficult to achieve by SLM methods due to the absence of mechanical pressure (as in conventional procedures) and the difficulty of laying an even powder layer . The porosity in the LaserCUSING manufactured part has a direct effect on the resulting mechanical properties. For instance, micro-flaws and voids serve as stress raisers for crack initiation, and vastly reduce fatigue performance [13,17]. Another concern with LaserCUSING processed Ti-6Al-4V is how the as-built mechanical properties compare with those of wrought forms. In particular, the fast cooling rates and layer-wise building in the LaserCUSING process result in a fine, non-equilibrium phase and anisotropic behaviour [16-20]. This martensitic microstructure manifests in high hardness and high strength/low ductility material behaviour, requiring the use of heat treatments to obtain a balance of properties similar to those of the bulk materials. Bracken et al.  revealed that heat treatments require tailoring to the as-built starting microstructure in
order to improve properties. So standard heat treatments such as mill, duplex, and beta annealing do not optimise LaserCUSING processed material performance. The above argument reveals that the industrial implementation of LaserCUSING Ti-6Al-4V products pivots on the characterisation of its as-built material behaviour, optimisation of processing parameters, and successful application of remedial post-processing. In this study, LaserCUSING processed Ti-6Al-4V is subjected to hardness evaluation, microstructural analysis, and density investigations. Focus is placed on the combination of machine parameters and heat treatments that will optimise material behaviour while minimising residual stresses and porosity defects.
2 EXPERIMENTAL METHODOLOGY
This study highlights the collective findings of Van Rooyen  and Khan  specifically related to the LaserCUSING process. The investigated material properties encompass the density, hardness, and microstructural detail. The effects of both SLM-tailored heat treatments are studied, together with the process parameter-dependence of the material porosity levels.
2.1 Specimen fabrication
The specimen base material selected was extra-low interstitial (ELI) Ti-6Al-4V powder, designated as CL 41 It (ELI). The Ti-6Al-4V ELI grade is a higher-purity version of Ti-6Al-4V, with lower amounts of iron impurities and carbon and oxygen interstitials . The lower oxygen content of this material makes it more suitable for fracture-critical aerospace, medical, and cryogenic applications . The powder particles, produced by gas atomisation, range from 38 to 45 m in size. All samples were produced on an M2 LaserCUSING machine in the Rapid Product Development Laboratory at the University of Stellenbosch. The machine is equipped with a 200W continuous wave fibre laser with a variable laser spot diameter. During fabrication, the build chamber is flushed with an argon atmosphere to prevent the oxidation of the titanium parts. The samples were built with 100W laser power, 30 m powder layer thickness, and a 150 m